Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

JOURNAL OF ENVIRONMENTAL HEALTH SCIENCE & ENGINEERING

RESEARCH ARTICLE

Open Access

Removal of reactive blue 19 from aqueous solution by pomegranate residual-based activated carbon: optimization by response surface methodology Elham Radaei1, Mohammad Reza Alavi Moghaddam1* and Mokhtar Arami2

Abstract Background: In this research, response surface methodology (RSM) was applied to optimize Reactive Blue 19 removal by activated carbon from pomegranate residual. A 24 full factorial central composite design (CCD) was applied to evaluate the effects of initial pH, adsorbent dose, initial dye concentration, and contact time on the dye removal efficiency. Methodology: The activated carbon prepared by 50 wt.% phosphoric acid activation under air condition at 500°C. The range of pH and initial dye concentration were selected in a way that considered a wide range of those variables. Furthermore, the range of contact time and adsorbent dose were determined based on initial tests. Levels of selected variables and 31 experiments were determined. MiniTab (version 16.1) was used for the regression and graphical analyses of the data obtained. Results: It was found that the decrease of initial dye concentration and the increase of initial pH, adsorbent dose, and contact time are beneficial for improving the dye removal efficiency. Analysis of variance (ANOVA) results presented high R2 value of 99.17% for Reactive Blue 19 dye removal, which indicates the accuracy of the polynomial model is acceptable. Conclusions: Initial pH of 11, adsorbent dose of 1.025 g/L, initial dye concentration of 100 mg/L, and contact time of 6.8 minutes found to be the optimum conditions. Dye removal efficiency of 98.7% was observed experimentally at optimum point which confirmed close to model predicted (98.1%) result. Keywords: Reactive dye, Adsorption, Pomegranate residual, Response surface methodology

Introduction Many industries, especially textile and food industries often use dyes and pigments to color their products. As a result, these industries often discharge large amounts of colored effluents due to unfixed dyes on fibres or food during coloring and washing steps [1]. Due to the disposal of these effluents into the receiving water body may cause severe damage to aquatic biota and humans due to mutagenic and carcinogenic effects [2-4], it is of great importance to provide waste-treatment facilities for minimizing these substances in the effluents before discharge.

There are several methods available for treatment of dye-containing wastewater, such as membrane [5], electrochemical [6], coagulation/flocculation [7], and biological [8]. The adsorption technique has been found not only to be effective, but also practical in application for the dye-containing wastewater treatment, due to its high efficiency, simplicity, ease of operation, and the availability of a wide range of adsorbents [9,10]. Activated carbons (ACs) are widely used as the most efficient adsorbents. The chemical activation is often used to produce ACs and it involves mixing the feedstock with a chemical activating agent such as H3PO4, ZnCl2, and KOH [11-13].

* Correspondence: [email protected] 1 Department of Civil and Environmental Engineering, Amirkabir University of Technology (AUT), Tehran, Iran Full list of author information is available at the end of the article © 2014 Radaei et al.; licensee BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Table 1 Chemical structure and characteristics of RB19 Characteristics

Values

Molecular formula

C22H16N2Na2O11S3

λmax (nm)

594

Molecular weight (MW)

626.54

Chemical structure

Conventional and classical methods of studying a process by maintaining other factors involved at an unspecified constant level does not depict the combined effect of all the factors involved. Response Surface Methodology (RSM) is a collection of mathematical and statistical techniques useful for developing, improving, and optimizing processes and can be used to evaluate the relative significance of several affecting factors even in the presence of complex interactions. The main objective of RSM is to determine the optimum operational conditions for the system or to determine a region that satisfies the operating specifications [14]. Many research groups applied this method for removal of different pollutants by adsorption process [14-19]. The aim of the present study is to optimize and model the removal of Reactive Blue 19 from aqueous solution by activated carbon derived from pomegranate residual using RSM. The relationship between dye removal efficiency and four main independent parameters including initial pH, initial dye concentration, adsorbent dose, and contact time were evaluated by applying central composite design (CCD).

Company and is widely used in textile industries in Iran. The chemical structure and characteristics of the selected dye is presented in Table 1. The solution pH measurement was carried out using a 340i/SET pH meter (WTW-Germany) and was adjusted by 1 M hydrochloric acid or 1 M sodium hydroxide. The dye solution and adsorbent was agitated by a jar test at 150 rpm agitation speed at ambient temperature 25°C. A six beaker jar test apparatus from Zag-Chemi Company in Iran was used to simulate the adsorption process. All samples were filtered through glass fibre filters GF/A. The clear supernatants were analyzed for RB19 dye concentrations using a UV–vis HACH spectrophotometer (DR/4000). In this study, pomegranate residual was collected from Meykhosh juice industry in Yazd/Iran. Pomegranate residual has been dried in an oven for 2 h at 100°C until a constant weight was reached. It was then ground in a ball mill and passed through sieve No.8. They were soaked for 24 h in the ratio of 1:1 (w/v) with 50 wt.% phosphoric acid at room temperature. The sample is then decanted, dried in a muffle furnace for 1 h at 500°C. Then the samples were washed sequentially several times with hot distilled water, until pH of the washing solution became neutral. In the last step, activated carbon (AC) was powder and sieved by the No. 200 mesh. The textural properties of adsorbent were also tested by N2 adsorption/desorption isotherms at 77 K using an Autosorb 1 analyzer (Quantachrome Corporation, USA). The specific surface area (SBET ) was calculated by Brun- auer–Emmett–Teller (BET) method. The textural characteristics of AC are shown in Table 2. The pore size distribution was determined by using the Barrett–Joyner– Halenda (BJH) method (Figure 1).

Methods Materials and activated carbon preparation

Dye solution was prepared by dissolving Reactive blue 19 (RB19) which was provided by the Alvan Sabet Table 2 Textural properties obtained by N2 adsorption/ desorption studies Parameters

Values

BET surface area (m2/g) 3

BETa

825.46 b

Pore volume (cm /g)

BJH adsorption

0.3455

Pore diameter (Å)

BJH adsorption

14.35

a

Computed in the P/P0 range 0.05–0.30. b BJH (Barrett Joyner Halenda) cumulative adsorption pore volume for pores in range of 0 and 5000 Å diameter.

Page 2 of 8

Figure 1 Pore size distribution of AC.

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Page 3 of 8

(a)

(b)

Figure 2 Results of initial tests for determining of adsorbent dose and contact time, initial pH = 11: (a) initial dye concentration = 300 mg/L and (b) initial dye concentration = 500 mg/L.

Table 4 RSM design and its observed and predicted values

Experimental design

A central composite design (CCD) was employed for determining the optimum condition for the dye removal. A total of 31 experiments were carried out according to a 24 full factorial CCD, consisting of 16 factorial experiments (coded to the usual ± 1 notation), 8 axial experiments (on the axis at a distance of ± α from the center), and 7 replicates (at the center of the experimental domain). The value of α for rotatability depends on the number of points in the factorial portion of the design, which is given in equation (1): α ¼ ðNF Þ1=4

ð1Þ

where NF is the number of points in the cube portion of the design (NF =2k, k is the number of factors). Therefore, α is equal to (24)1/4 = 2 according to equation (1). The range of pH and initial dye concentration were selected in a way that considered a wide range of those variables. The dye concentration was selected between 100 to 500 mg/L. This range is based on determined actual concentration of textile wastewaters in Iran. The range of contact time and adsorbent dose were determined based on initial tests. The results of initial tests are shown in Figure 2. As demonstrated in the figures,

Table 3 Experimental range and levels of the independent variables Parameters

Levels

Initial dye Contact Dye removal (%) Run Initial Adsorbent dose concentration time pH Experimental Predicted (x2) (x3) (x4) (x1) 1

5

1

200

3

70.46

70.99

2 3

9

1

200

3

71.57

72.39

5

1.5

200

3

89.35

87.55

4

9

1.5

200

3

91.64

92.28

5

5

1

400

3

49.39

47.68

6

9

1

400

3

51.40

52.31

7

5

1.5

400

3

64.34

64.06

8

9

1.5

400

3

72.00

72.01

9

5

1

200

7

73.06

73.08

10

9

1

200

7

74.41

74.71

11

5

1.5

200

7

90.54

89.65

12

9

1.5

200

7

92.84

94.59

13

5

1

400

7

50.87

50.25

14

9

1

400

7

53.28

55.11

15

5

1.5

400

7

67.43

66.63

16

9

1.5

400

7

75.32

74.80

17

3

1.25

300

5

75.98

78.77

18

11

1.25

300

5

91.19

88.35

19

7

0.75

300

5

45.68

44.66

20

7

1.75

300

5

79.95

80.92

21

7

1.25

100

5

93.52

92.87

22

7

1.25

500

5

49.17

49.78

23

7

1.25

300

1

63.94

64.40

24

7

1.25

300

9

69.80

69.29

25

7

1.25

300

5

69.27

69.33

26

7

1.25

300

5

70.50

69.33

-α

-1

0

1

α

27

7

1.25

300

5

69.27

69.33

Initial pH

x1

3

5

7

9

11

28

7

1.25

300

5

68.30

69.33

Adsorbent dose (g/L)

x2

0.75

1.00

1.25

1.50

1.75

29

7

1.25

300

5

71.27

69.33

Initial dye concentration (mg/L)

x3

100

200

300

400

500

30

7

1.25

300

5

67.47

69.33

Contact time (min)

x4

1

3

5

7

9

31

7

1.25

300

5

69.27

69.33

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Table 5 Statistical regression coefficients for RB19 removal efficiency (%) in coded units Term

Page 4 of 8

The behavior of the adsorption process is explained by the following empirical second-order polynomial model equation (3):

Coefficient

SE Coefficient

T

P

Constant

69.3371

0.6393

108.465

0.000

x1

2.3943

0.3452

6.935

0.000

x2

9.0655

0.3452

26.259

0.000

x3

−10.7734

0.3452

−31.206

0.000

x4

1.2223

0.3452

3.541

0.003

x21

3.5562

0.3163

11.244

0.000

x22

−1.6346

0.3163

−5.168

0.000

x23

0.4977

0.3163

1.573

0.135

x24

−0.6212

0.3163

−1.964

0.067

x1x2

0.8284

0.4228

1.959

0.068

x1x3

0.8070

0.4228

1.909

0.074

x1x4

0.0549

0.4228

0.130

0.898

Results

x2x3

−0.0465

0.4228

−0.110

0.914

Statistical analysis

x2x4

−0.0007

0.4228

−0.002

0.999

x3x4

0.1210

0.4228

0.286

0.778

The experimental design matrix, the experimental results and the predicted dye removal efficiency are presented in Table 4. The final model is expressed by equation (4):

the dye was rapidly adsorbed at a high rate in the first 5 minute, and after 10 minutes leveled off. Therefore, the range of contact time was considered between 1 minute and 10 minutes. Due to a slight difference between dye removal efficiencies for adsorbent dose of 2 g/L and 1.75 g/L, the maximum amount of adsorbent dose was considered 1.75 g/L. In addition, adsorbent dose of lower than 0.75 g/L was not enough efficient to remove RB19. Levels of selected variables are presented in Table 3. For statistical calculations, the variables Xi (the real value of an independent variable) were coded as xi (dimensionless value of an independent variable) according to equation (2): xi ¼ ðXi –X0 Þ=ΔX

ð2Þ

where X0 is the value of Xi at the center point and ΔX represents the step change. Table 6 ANOVA for RB19 removal efficiency (%) Source

DF

Seq SS

Adj SS

Adj MS

F

P

Regression

14

5455.27

5455.27

389.66

136.22

0.000

Linear

4

4931.44

4931.44

1232.86

430.99

0.000

Square

4

502.12

502.12

125.53

43.88

0.000

Interaction

6

21.72

21.72

3.62

1.27

0.327

Residual error

16

45.77

45.77

2.86

Lack-of-fit

10

36.11

36.11

3.61

2.24

0.168

9.66

1.61

Pure error

6

9.66

Total

30

5501.04

Note: R2 = 99.17%, R2 (adj) = 98.44%.

Yi ¼ b0 þ

n X i¼1

bi x i þ

n X i¼1

bii xi 2 þ

n‐1 X n X

bij xi xj

ð3Þ

i¼1 j¼iþ1

where Y is the predicted response (dye removal efficiency), b0 the constant coefficient, bi the linear coefficients, bii the quadratic coefficients, bij the interaction coefficients and xi, xj are the coded values of the variables. MiniTab (version 16.1) was used for the regression and graphical analyses of the data obtained. The reliability of the fitted model was justified through ANOVA and the coefficient of R2.

Y ¼ 69:3371 þ 2:3943 x1 þ 9:0655 x2 ‐10:7734x3 þ 1:2223 x4 þ 3:5562x1 2 ‐1:6346x2 2 þ 0:4977 x3 2 ‐0:6212x4 2 þ 0:8284x1 x2 þ 0:8070 x1 x3 þ 0:0549 x1 x4 ‐0:0465x2 x3 ‐0:0007x2 x4 þ 0:1210 x3 x4

ð4Þ

Statistical regression coefficients for RB19 dye removal efficiency (%) is provided in Table 5. Amounts of P (P < 0.05) for all independent parameters confirms that four selected factors are significant. However, it was found that all square and interaction terms except x21 and x22 (P values of 0.000) were insignificant to the response. ANOVA for the selected dye removal is also listed in Table 6. In this case, the P-value of 0.000 (P < 0.05) for regression model equation implies that the second-order polynomial model fitted to the experimental results well. The lack-of-fit was also calculated from the experimental error (pure error) and residuals. “F-value of Lack-of-fit” of 2.24 implies the significance of model correlation between the variables and process response for dye removal. Additionally, the value of R 2 = 99.17% and R2 (adj) =98.44% confirm the accuracy of the model. Furthermore, parity plot for the experimental and predicted value of RB19 removal efficiency (%) is demonstrated in Figure 3. In addition, normal probability and residuals versus fitted values plots for RB19 removal efficiency are illustrated in Figure 4. Normal probability plot is a suitable graphical method for judging the normality of the residuals [18]. As seen in Figure 4(a), the

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Page 5 of 8

Figure 3 Parity plot for the experimental and predicted value of RB19 removal efficiency (%).

Figure 5(a, b, c), by increasing of initial pH and adsorbent dose, and decreasing of initial dye concentration, the dye removal efficiency improved. Moreover, as shown in Figure 5(d), adsorption efficiency rapidly increased with an increase in contact time within the first minutes. Then, the rate of adsorption was found to be relatively slow and then constant. As shown in this Figure, the dye removal is highly dependent on adsorbent dose and initial dye concentration, and the initial pH and contact time slightly influenced the process efficiency. For a better explanation of the independent variables and their interactive effects on the dye removal, 3D plots and its corresponding contour plots are represented in Figure 6. At constant value of the initial dye concentration (300 mg/L), when the adsorbent

normality assumption was relatively satisfied as the points in the plot form a fairly straight line. The reliability of the model was also examined with the plot of residuals versus fits in Figure 4(b). As Figure 4(b) shows, the number of increasing or decreasing points was significantly close; patterns of increasing residuals and increasing fits were similar; and, positive and negative residuals were scattered in same range. As a result, Figure 4 shows that the model is adequate to describe RB19 removal efficiency by response surface methodology for AC. Response surface and counter plotting for evaluation of operational parameters

The main effect of each parameter on the dye removal efficiency is showed in Figure 5. As illustrated in

Residuals Versus the Fitted Values

Normal Probability Plotof the Residuals 99

3

95

2

80 70 60 50 40 30 20

1 Residual

Percent

90

0 -1

10 5

-2 -3

1 -3

-2

-1

0

1

2

3

40

50

60

Residual

(a) Figure 4 (a) Normal probability plot and (b) residual versus fit plot for RB19 removal efficiency (%).

70

Fitted Value

(b)

80

90

100

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Page 6 of 8

Data Means

(a)

(b)

Initial pH

Adsorbent dose(g/L)

90

Mean of dye removal (% )

80 70 60 50 3

5

7

9

11

(c) Initial dye concentration(mg/L)

0.75

(d)

1.00 1.25 1.50 Contact time(min)

1.75

90 80 70 60 50 100

200

300

400

500

1

3

5

7

9

Figure 5 Main effect plots of parameters for RB19 removal efficiency: (a) initial pH, (b) adsorbent dose, (c) initial dye concentration and (d) contact time.

dose and initial pH increase, the dye removal efficiency increases and finally reaches to 100% (Figure 6 (a)). Moreover, for given initial dye concentration of 100 mg/L and adsorbent dose of 1.25 g/L, dye removal efficiency is almost independent of initial pH (Figure 6(b)). This independency is due to the existence of numerous active sites for the adsorption, whereas the independency was decreased with increasing of initial dye concentration. As shown in Figure 6(c), there are no significant changes on the dye removal surface with the increase of contact time and initial pH.

Process optimization

In order to determine the optimum conditions by the adsorption process, the desired aim in terms of RB19 removal efficiency was defined as target to achieve 98% removal efficiency. The optimum values of the process parameters were calculated in coded units (xi) and then converted into uncoded units (Xi) using Equation (1). Initial pH of 11, adsorbent dose of 1.025 g/L, initial dye concentration of 100 mg/L and contact time of 6.8 minutes found to be the optimum conditions by the model. The optimum condition was repeated three times and dye removal efficiencies of 98.4, 98.6, and 99.1% were resulted. The average of 98.7% dye removal efficiency was found close to the model prediction of 98.1%.

Discussion According to the results, contact time is the least important parameter, which is reported by other research groups [20,21]. Furthermore, by increasing of initial pH and adsorbent dose, and decreasing of initial dye concentration, the dye removal efficiency improved. These results are in good agreement with of previous studies [22,23]. The effect of the four selected independent parameters and interactions among the RSM were analyzed which was shown that some interactions like (x 21 and x 22) influenced the adsorption performance as well as all selected parameters. ANOVA showed a high R 2 value of regressions model equation (R2 = 0.9917), thus ensuring a satisfactory adjustment of the second-order regression model with the experimental data. The optimum RB19 removal efficiency were found at initial pH of 11, adsorbent dose of 1.025 g/L, initial dye concentration of 100 mg/l and contact time of 6.8 min. An experiment was performed in optimum conditions which confirmed that the model and experimental results are in close agreement (98.7% compared to 98.1% for the model). Conclusions In this research, response surface methodology was applied as an experimental design to explore the optimal conditions for RB19 dye removal from aqueous solutions by activated carbon prepared by pomegranate

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Page 7 of 8

Figure 6 Surface corresponding contour plot as a function of initial pH and: (a) adsorbent dose (initial dye concentration of 300 mg/l and contact time of 5 min) (b) initial dye concentration (adsorbent dose of 1.25 g/L and contact time of 5 min) (c) contact time (initial dye concentration of 300 mg/l and adsorbent dose of 1.25 g/L).

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

residual. The effect of four operating variables of adsorption process including initial pH, adsorbent dose, initial dye concentration, and contact time were examined. The BET method showed that the average SBET of AC was 825.46 m2 g−1. The results of this investigation presented that RSM is a powerful statistical optimization and modeling tool for RB19 removal using adsorption process. Competing interests The authors declare that they have no competing interests. Authors’ contributions This work is part of the Master thesis of ER where MRA, Supervisor of the thesis, suggested the problem and read the paper and MR, Co-Supervisor of the thesis, helped in analysis of experiments. All authors read and approved the final manuscript. Acknowledgements The authors are grateful to the Amirkabir University of Technology (AUT) research fund for the financial support. In addition, the authors wish to express thanks to Ms. Armineh Azizi and Ms. Shabnam Sadri Moghaddam (PhD students of environmental engineering), and Ms. Lida Ezzedinloo for their assistance during experiments. Author details 1 Department of Civil and Environmental Engineering, Amirkabir University of Technology (AUT), Tehran, Iran. 2Department of Textile Engineering, Amirkabir University of Technology (AUT), Tehran, Iran. Received: 27 December 2012 Accepted: 5 March 2014 Published: 28 March 2014 References 1. Santos SCR, Boaventura RAR: Adsorption modeling of textile dyes by sepiolite. Appl Clay Sci 2008, 42:137–145. 2. Crini G: Non-conventional low-cost adsorbents for dye removal: a review. Bioresour Technol 2006, 97:1061–1085. 3. Sadri MS, Alavi Moghaddam MR, Arami M: Decolorization of an acidic dye from synthetic wastewater by sludge of water treatment plant. Iran J Environ Health Sci Eng 2010, 7:437–442. 4. Ehrampoush MH, Ghanizadeh G, Ghaneian MT: Equilibrium and kinetics study of reactive red 123 dye removal from aqueous solution by adsorption on eggshell. Iran J Environ Health Sci Eng 2011, 8:101–108. 5. Xu Y, Lebrun RE: Treatment of textile dye plant effluent by nanofiltration membrane. Separa Sci Technol 1999, 34:2501–2519. 6. Bechtold T, Burtscher E, Turcanu A: Cathodic decolorisation of textile wastewater containing reactive dyes using multi-cathode electrolyser. J Chem Technol Biotechnol 2001, 76:303–311. 7. Sadri MS, Alavi Moghaddam MR, Arami M: Coagulation/flocculation process for dye removal using sludge from water treatment plant: optimization through response surface methodology. J Hazard Mater 2010, 175:651–657. 8. Hosseini KE, Alavi Moghaddam MR, Hashemi SH: Investigation of decolorization kinetics and biodegradation of azo dye Acid Red 18 using sequential process of anaerobic sequencing batch reactor/moving bed sequencing batch biofilm reactor. Int Biodeter Biodeg 2012, 71:43–49. 9. Chatterjee S, Lee DS, Lee MW, Woo SH: Enhanced adsorption of congo red from aqueous solutions by chitosan hydrogel beads impregnated with cetyl trimethyl ammonium bromide. Bioresour Technol 2009, 100:2803–2809. 10. Samarghandi MR, Zarrabi M, Noori Sepehr M, Amrane A, Hossein Safari G, Bashiri S: Application of acidic treated pumice as an adsorbent for the removal of azo dye from aqueous solutions: kinetic, equilibrium and thermodynamic studies. Iran J Environ Health Sci Eng 2012, 9:101–108. 11. Lua AC, Yang T: Characteristics of activated carbon prepared from pistachio-nut shell by zinc chloride activation under nitrogen and vacuum conditions. J Colloid Inter Sci 2005, 290:505–513. 12. Benadjemia M, Millière L, Reinert L, Benderdouche N, Duclaux L: Preparation, characterization and Methylene Blue adsorption of phosphoric acid activated carbons from globe artichoke leaves. Fuel Process Technol 2011, 92:1203–1212.

Page 8 of 8

13. Wu FC, Wu PH, Tseng RL, Juang RS: Preparation of activated carbons from unburnt coal in bottom ash with KOH activation for liquid-phase adsorption. J Environ Manage 2010, 91:1097–1102. 14. Ravikumar K, Ramalingam S, Krishnan S, Balu K: Application of response surface methodology to optimize the process variables for reactive red and acid brown dye removal using a novel adsorbent. Dyes Pigment 2006, 70:18–26. 15. Auta M, Hameed BH: Optimized waste tea activated carbon for adsorption of methylene blue and acid blue 29 dyes using response surface methodology. Chem Eng J 2011, 175:233–243. 16. Liu Y, Wang J, Zheng Y, Wang A: Adsorption of methylene blue by kapok fiber treated by sodium chlorite optimized with response surface methodology. Chem Eng J 2012, 184:248–255. 17. Chatterjee S, Kumar A, Basu S, Dutta S: Application of response surface methodology for methylene blue dye removal from aqueous solution using low cost adsorbent. Chem Eng J 2012, 181:289–299. 18. Azizi A, Alavi Moghaddam MR, Arami M: Application of wood waste for a reactive dye removal from aqueous solutions: optimization through response surface methodology. J Environ Eng Manag. in press. 19. Liu Y, Zheng Y, Wang A: Response surface methodology for optimizing adsorption process parameters for methylene blue removal by a hydrogel composite. Adsorp Sci Technol 2010, 28:913–922. 20. Azizi A, Alavi Moghaddam MR, Arami M: Wood Waste from mazandaran wood and the paper industry as a low cost adsorbent for removal of a reactive dye. J Resid Sci Technol 2011, 8:21–28. 21. Khaled A, Nemr AE, Sikaily AE, Abdelwahab O: Removal of direct N blue106 from artificial textile dye effluent using activated carbon from orange peel: adsorption isotherm and kinetic studies. J Hazard Mater 2009, 165:100–110. 22. Mahmoodi NM, Hayati B, Arami M, Lan C: Adsorption of textile dyes on pine cone from colored wastewater: kinetic, equilibrium and thermodynamic studies. Desalination 2011, 268:117–125. 23. Sadri MS, Alavi Moghaddam MR, Aram M: A comparative study of acid red 119 dye adsorption onto dried sewage sludge and sewage sludge ash: isotherm, kinetic and desorption study. J Resid Sci Technol 2010, 7:199–207. doi:10.1186/2052-336X-12-65 Cite this article as: Radaei et al.: Removal of reactive blue 19 from aqueous solution by pomegranate residual-based activated carbon: optimization by response surface methodology. Journal of Environmental Health Science & Engineering 2014 12:65.

Submit your next manuscript to BioMed Central and take full advantage of: • Convenient online submission • Thorough peer review • No space constraints or color ﬁgure charges • Immediate publication on acceptance • Inclusion in PubMed, CAS, Scopus and Google Scholar • Research which is freely available for redistribution Submit your manuscript at www.biomedcentral.com/submit

JOURNAL OF ENVIRONMENTAL HEALTH SCIENCE & ENGINEERING

RESEARCH ARTICLE

Open Access

Removal of reactive blue 19 from aqueous solution by pomegranate residual-based activated carbon: optimization by response surface methodology Elham Radaei1, Mohammad Reza Alavi Moghaddam1* and Mokhtar Arami2

Abstract Background: In this research, response surface methodology (RSM) was applied to optimize Reactive Blue 19 removal by activated carbon from pomegranate residual. A 24 full factorial central composite design (CCD) was applied to evaluate the effects of initial pH, adsorbent dose, initial dye concentration, and contact time on the dye removal efficiency. Methodology: The activated carbon prepared by 50 wt.% phosphoric acid activation under air condition at 500°C. The range of pH and initial dye concentration were selected in a way that considered a wide range of those variables. Furthermore, the range of contact time and adsorbent dose were determined based on initial tests. Levels of selected variables and 31 experiments were determined. MiniTab (version 16.1) was used for the regression and graphical analyses of the data obtained. Results: It was found that the decrease of initial dye concentration and the increase of initial pH, adsorbent dose, and contact time are beneficial for improving the dye removal efficiency. Analysis of variance (ANOVA) results presented high R2 value of 99.17% for Reactive Blue 19 dye removal, which indicates the accuracy of the polynomial model is acceptable. Conclusions: Initial pH of 11, adsorbent dose of 1.025 g/L, initial dye concentration of 100 mg/L, and contact time of 6.8 minutes found to be the optimum conditions. Dye removal efficiency of 98.7% was observed experimentally at optimum point which confirmed close to model predicted (98.1%) result. Keywords: Reactive dye, Adsorption, Pomegranate residual, Response surface methodology

Introduction Many industries, especially textile and food industries often use dyes and pigments to color their products. As a result, these industries often discharge large amounts of colored effluents due to unfixed dyes on fibres or food during coloring and washing steps [1]. Due to the disposal of these effluents into the receiving water body may cause severe damage to aquatic biota and humans due to mutagenic and carcinogenic effects [2-4], it is of great importance to provide waste-treatment facilities for minimizing these substances in the effluents before discharge.

There are several methods available for treatment of dye-containing wastewater, such as membrane [5], electrochemical [6], coagulation/flocculation [7], and biological [8]. The adsorption technique has been found not only to be effective, but also practical in application for the dye-containing wastewater treatment, due to its high efficiency, simplicity, ease of operation, and the availability of a wide range of adsorbents [9,10]. Activated carbons (ACs) are widely used as the most efficient adsorbents. The chemical activation is often used to produce ACs and it involves mixing the feedstock with a chemical activating agent such as H3PO4, ZnCl2, and KOH [11-13].

* Correspondence: [email protected] 1 Department of Civil and Environmental Engineering, Amirkabir University of Technology (AUT), Tehran, Iran Full list of author information is available at the end of the article © 2014 Radaei et al.; licensee BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Table 1 Chemical structure and characteristics of RB19 Characteristics

Values

Molecular formula

C22H16N2Na2O11S3

λmax (nm)

594

Molecular weight (MW)

626.54

Chemical structure

Conventional and classical methods of studying a process by maintaining other factors involved at an unspecified constant level does not depict the combined effect of all the factors involved. Response Surface Methodology (RSM) is a collection of mathematical and statistical techniques useful for developing, improving, and optimizing processes and can be used to evaluate the relative significance of several affecting factors even in the presence of complex interactions. The main objective of RSM is to determine the optimum operational conditions for the system or to determine a region that satisfies the operating specifications [14]. Many research groups applied this method for removal of different pollutants by adsorption process [14-19]. The aim of the present study is to optimize and model the removal of Reactive Blue 19 from aqueous solution by activated carbon derived from pomegranate residual using RSM. The relationship between dye removal efficiency and four main independent parameters including initial pH, initial dye concentration, adsorbent dose, and contact time were evaluated by applying central composite design (CCD).

Company and is widely used in textile industries in Iran. The chemical structure and characteristics of the selected dye is presented in Table 1. The solution pH measurement was carried out using a 340i/SET pH meter (WTW-Germany) and was adjusted by 1 M hydrochloric acid or 1 M sodium hydroxide. The dye solution and adsorbent was agitated by a jar test at 150 rpm agitation speed at ambient temperature 25°C. A six beaker jar test apparatus from Zag-Chemi Company in Iran was used to simulate the adsorption process. All samples were filtered through glass fibre filters GF/A. The clear supernatants were analyzed for RB19 dye concentrations using a UV–vis HACH spectrophotometer (DR/4000). In this study, pomegranate residual was collected from Meykhosh juice industry in Yazd/Iran. Pomegranate residual has been dried in an oven for 2 h at 100°C until a constant weight was reached. It was then ground in a ball mill and passed through sieve No.8. They were soaked for 24 h in the ratio of 1:1 (w/v) with 50 wt.% phosphoric acid at room temperature. The sample is then decanted, dried in a muffle furnace for 1 h at 500°C. Then the samples were washed sequentially several times with hot distilled water, until pH of the washing solution became neutral. In the last step, activated carbon (AC) was powder and sieved by the No. 200 mesh. The textural properties of adsorbent were also tested by N2 adsorption/desorption isotherms at 77 K using an Autosorb 1 analyzer (Quantachrome Corporation, USA). The specific surface area (SBET ) was calculated by Brun- auer–Emmett–Teller (BET) method. The textural characteristics of AC are shown in Table 2. The pore size distribution was determined by using the Barrett–Joyner– Halenda (BJH) method (Figure 1).

Methods Materials and activated carbon preparation

Dye solution was prepared by dissolving Reactive blue 19 (RB19) which was provided by the Alvan Sabet Table 2 Textural properties obtained by N2 adsorption/ desorption studies Parameters

Values

BET surface area (m2/g) 3

BETa

825.46 b

Pore volume (cm /g)

BJH adsorption

0.3455

Pore diameter (Å)

BJH adsorption

14.35

a

Computed in the P/P0 range 0.05–0.30. b BJH (Barrett Joyner Halenda) cumulative adsorption pore volume for pores in range of 0 and 5000 Å diameter.

Page 2 of 8

Figure 1 Pore size distribution of AC.

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Page 3 of 8

(a)

(b)

Figure 2 Results of initial tests for determining of adsorbent dose and contact time, initial pH = 11: (a) initial dye concentration = 300 mg/L and (b) initial dye concentration = 500 mg/L.

Table 4 RSM design and its observed and predicted values

Experimental design

A central composite design (CCD) was employed for determining the optimum condition for the dye removal. A total of 31 experiments were carried out according to a 24 full factorial CCD, consisting of 16 factorial experiments (coded to the usual ± 1 notation), 8 axial experiments (on the axis at a distance of ± α from the center), and 7 replicates (at the center of the experimental domain). The value of α for rotatability depends on the number of points in the factorial portion of the design, which is given in equation (1): α ¼ ðNF Þ1=4

ð1Þ

where NF is the number of points in the cube portion of the design (NF =2k, k is the number of factors). Therefore, α is equal to (24)1/4 = 2 according to equation (1). The range of pH and initial dye concentration were selected in a way that considered a wide range of those variables. The dye concentration was selected between 100 to 500 mg/L. This range is based on determined actual concentration of textile wastewaters in Iran. The range of contact time and adsorbent dose were determined based on initial tests. The results of initial tests are shown in Figure 2. As demonstrated in the figures,

Table 3 Experimental range and levels of the independent variables Parameters

Levels

Initial dye Contact Dye removal (%) Run Initial Adsorbent dose concentration time pH Experimental Predicted (x2) (x3) (x4) (x1) 1

5

1

200

3

70.46

70.99

2 3

9

1

200

3

71.57

72.39

5

1.5

200

3

89.35

87.55

4

9

1.5

200

3

91.64

92.28

5

5

1

400

3

49.39

47.68

6

9

1

400

3

51.40

52.31

7

5

1.5

400

3

64.34

64.06

8

9

1.5

400

3

72.00

72.01

9

5

1

200

7

73.06

73.08

10

9

1

200

7

74.41

74.71

11

5

1.5

200

7

90.54

89.65

12

9

1.5

200

7

92.84

94.59

13

5

1

400

7

50.87

50.25

14

9

1

400

7

53.28

55.11

15

5

1.5

400

7

67.43

66.63

16

9

1.5

400

7

75.32

74.80

17

3

1.25

300

5

75.98

78.77

18

11

1.25

300

5

91.19

88.35

19

7

0.75

300

5

45.68

44.66

20

7

1.75

300

5

79.95

80.92

21

7

1.25

100

5

93.52

92.87

22

7

1.25

500

5

49.17

49.78

23

7

1.25

300

1

63.94

64.40

24

7

1.25

300

9

69.80

69.29

25

7

1.25

300

5

69.27

69.33

26

7

1.25

300

5

70.50

69.33

-α

-1

0

1

α

27

7

1.25

300

5

69.27

69.33

Initial pH

x1

3

5

7

9

11

28

7

1.25

300

5

68.30

69.33

Adsorbent dose (g/L)

x2

0.75

1.00

1.25

1.50

1.75

29

7

1.25

300

5

71.27

69.33

Initial dye concentration (mg/L)

x3

100

200

300

400

500

30

7

1.25

300

5

67.47

69.33

Contact time (min)

x4

1

3

5

7

9

31

7

1.25

300

5

69.27

69.33

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Table 5 Statistical regression coefficients for RB19 removal efficiency (%) in coded units Term

Page 4 of 8

The behavior of the adsorption process is explained by the following empirical second-order polynomial model equation (3):

Coefficient

SE Coefficient

T

P

Constant

69.3371

0.6393

108.465

0.000

x1

2.3943

0.3452

6.935

0.000

x2

9.0655

0.3452

26.259

0.000

x3

−10.7734

0.3452

−31.206

0.000

x4

1.2223

0.3452

3.541

0.003

x21

3.5562

0.3163

11.244

0.000

x22

−1.6346

0.3163

−5.168

0.000

x23

0.4977

0.3163

1.573

0.135

x24

−0.6212

0.3163

−1.964

0.067

x1x2

0.8284

0.4228

1.959

0.068

x1x3

0.8070

0.4228

1.909

0.074

x1x4

0.0549

0.4228

0.130

0.898

Results

x2x3

−0.0465

0.4228

−0.110

0.914

Statistical analysis

x2x4

−0.0007

0.4228

−0.002

0.999

x3x4

0.1210

0.4228

0.286

0.778

The experimental design matrix, the experimental results and the predicted dye removal efficiency are presented in Table 4. The final model is expressed by equation (4):

the dye was rapidly adsorbed at a high rate in the first 5 minute, and after 10 minutes leveled off. Therefore, the range of contact time was considered between 1 minute and 10 minutes. Due to a slight difference between dye removal efficiencies for adsorbent dose of 2 g/L and 1.75 g/L, the maximum amount of adsorbent dose was considered 1.75 g/L. In addition, adsorbent dose of lower than 0.75 g/L was not enough efficient to remove RB19. Levels of selected variables are presented in Table 3. For statistical calculations, the variables Xi (the real value of an independent variable) were coded as xi (dimensionless value of an independent variable) according to equation (2): xi ¼ ðXi –X0 Þ=ΔX

ð2Þ

where X0 is the value of Xi at the center point and ΔX represents the step change. Table 6 ANOVA for RB19 removal efficiency (%) Source

DF

Seq SS

Adj SS

Adj MS

F

P

Regression

14

5455.27

5455.27

389.66

136.22

0.000

Linear

4

4931.44

4931.44

1232.86

430.99

0.000

Square

4

502.12

502.12

125.53

43.88

0.000

Interaction

6

21.72

21.72

3.62

1.27

0.327

Residual error

16

45.77

45.77

2.86

Lack-of-fit

10

36.11

36.11

3.61

2.24

0.168

9.66

1.61

Pure error

6

9.66

Total

30

5501.04

Note: R2 = 99.17%, R2 (adj) = 98.44%.

Yi ¼ b0 þ

n X i¼1

bi x i þ

n X i¼1

bii xi 2 þ

n‐1 X n X

bij xi xj

ð3Þ

i¼1 j¼iþ1

where Y is the predicted response (dye removal efficiency), b0 the constant coefficient, bi the linear coefficients, bii the quadratic coefficients, bij the interaction coefficients and xi, xj are the coded values of the variables. MiniTab (version 16.1) was used for the regression and graphical analyses of the data obtained. The reliability of the fitted model was justified through ANOVA and the coefficient of R2.

Y ¼ 69:3371 þ 2:3943 x1 þ 9:0655 x2 ‐10:7734x3 þ 1:2223 x4 þ 3:5562x1 2 ‐1:6346x2 2 þ 0:4977 x3 2 ‐0:6212x4 2 þ 0:8284x1 x2 þ 0:8070 x1 x3 þ 0:0549 x1 x4 ‐0:0465x2 x3 ‐0:0007x2 x4 þ 0:1210 x3 x4

ð4Þ

Statistical regression coefficients for RB19 dye removal efficiency (%) is provided in Table 5. Amounts of P (P < 0.05) for all independent parameters confirms that four selected factors are significant. However, it was found that all square and interaction terms except x21 and x22 (P values of 0.000) were insignificant to the response. ANOVA for the selected dye removal is also listed in Table 6. In this case, the P-value of 0.000 (P < 0.05) for regression model equation implies that the second-order polynomial model fitted to the experimental results well. The lack-of-fit was also calculated from the experimental error (pure error) and residuals. “F-value of Lack-of-fit” of 2.24 implies the significance of model correlation between the variables and process response for dye removal. Additionally, the value of R 2 = 99.17% and R2 (adj) =98.44% confirm the accuracy of the model. Furthermore, parity plot for the experimental and predicted value of RB19 removal efficiency (%) is demonstrated in Figure 3. In addition, normal probability and residuals versus fitted values plots for RB19 removal efficiency are illustrated in Figure 4. Normal probability plot is a suitable graphical method for judging the normality of the residuals [18]. As seen in Figure 4(a), the

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Page 5 of 8

Figure 3 Parity plot for the experimental and predicted value of RB19 removal efficiency (%).

Figure 5(a, b, c), by increasing of initial pH and adsorbent dose, and decreasing of initial dye concentration, the dye removal efficiency improved. Moreover, as shown in Figure 5(d), adsorption efficiency rapidly increased with an increase in contact time within the first minutes. Then, the rate of adsorption was found to be relatively slow and then constant. As shown in this Figure, the dye removal is highly dependent on adsorbent dose and initial dye concentration, and the initial pH and contact time slightly influenced the process efficiency. For a better explanation of the independent variables and their interactive effects on the dye removal, 3D plots and its corresponding contour plots are represented in Figure 6. At constant value of the initial dye concentration (300 mg/L), when the adsorbent

normality assumption was relatively satisfied as the points in the plot form a fairly straight line. The reliability of the model was also examined with the plot of residuals versus fits in Figure 4(b). As Figure 4(b) shows, the number of increasing or decreasing points was significantly close; patterns of increasing residuals and increasing fits were similar; and, positive and negative residuals were scattered in same range. As a result, Figure 4 shows that the model is adequate to describe RB19 removal efficiency by response surface methodology for AC. Response surface and counter plotting for evaluation of operational parameters

The main effect of each parameter on the dye removal efficiency is showed in Figure 5. As illustrated in

Residuals Versus the Fitted Values

Normal Probability Plotof the Residuals 99

3

95

2

80 70 60 50 40 30 20

1 Residual

Percent

90

0 -1

10 5

-2 -3

1 -3

-2

-1

0

1

2

3

40

50

60

Residual

(a) Figure 4 (a) Normal probability plot and (b) residual versus fit plot for RB19 removal efficiency (%).

70

Fitted Value

(b)

80

90

100

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Page 6 of 8

Data Means

(a)

(b)

Initial pH

Adsorbent dose(g/L)

90

Mean of dye removal (% )

80 70 60 50 3

5

7

9

11

(c) Initial dye concentration(mg/L)

0.75

(d)

1.00 1.25 1.50 Contact time(min)

1.75

90 80 70 60 50 100

200

300

400

500

1

3

5

7

9

Figure 5 Main effect plots of parameters for RB19 removal efficiency: (a) initial pH, (b) adsorbent dose, (c) initial dye concentration and (d) contact time.

dose and initial pH increase, the dye removal efficiency increases and finally reaches to 100% (Figure 6 (a)). Moreover, for given initial dye concentration of 100 mg/L and adsorbent dose of 1.25 g/L, dye removal efficiency is almost independent of initial pH (Figure 6(b)). This independency is due to the existence of numerous active sites for the adsorption, whereas the independency was decreased with increasing of initial dye concentration. As shown in Figure 6(c), there are no significant changes on the dye removal surface with the increase of contact time and initial pH.

Process optimization

In order to determine the optimum conditions by the adsorption process, the desired aim in terms of RB19 removal efficiency was defined as target to achieve 98% removal efficiency. The optimum values of the process parameters were calculated in coded units (xi) and then converted into uncoded units (Xi) using Equation (1). Initial pH of 11, adsorbent dose of 1.025 g/L, initial dye concentration of 100 mg/L and contact time of 6.8 minutes found to be the optimum conditions by the model. The optimum condition was repeated three times and dye removal efficiencies of 98.4, 98.6, and 99.1% were resulted. The average of 98.7% dye removal efficiency was found close to the model prediction of 98.1%.

Discussion According to the results, contact time is the least important parameter, which is reported by other research groups [20,21]. Furthermore, by increasing of initial pH and adsorbent dose, and decreasing of initial dye concentration, the dye removal efficiency improved. These results are in good agreement with of previous studies [22,23]. The effect of the four selected independent parameters and interactions among the RSM were analyzed which was shown that some interactions like (x 21 and x 22) influenced the adsorption performance as well as all selected parameters. ANOVA showed a high R 2 value of regressions model equation (R2 = 0.9917), thus ensuring a satisfactory adjustment of the second-order regression model with the experimental data. The optimum RB19 removal efficiency were found at initial pH of 11, adsorbent dose of 1.025 g/L, initial dye concentration of 100 mg/l and contact time of 6.8 min. An experiment was performed in optimum conditions which confirmed that the model and experimental results are in close agreement (98.7% compared to 98.1% for the model). Conclusions In this research, response surface methodology was applied as an experimental design to explore the optimal conditions for RB19 dye removal from aqueous solutions by activated carbon prepared by pomegranate

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

Page 7 of 8

Figure 6 Surface corresponding contour plot as a function of initial pH and: (a) adsorbent dose (initial dye concentration of 300 mg/l and contact time of 5 min) (b) initial dye concentration (adsorbent dose of 1.25 g/L and contact time of 5 min) (c) contact time (initial dye concentration of 300 mg/l and adsorbent dose of 1.25 g/L).

Radaei et al. Journal of Environmental Health Science & Engineering 2014, 12:65 http://www.ijehse.com/content/12/1/65

residual. The effect of four operating variables of adsorption process including initial pH, adsorbent dose, initial dye concentration, and contact time were examined. The BET method showed that the average SBET of AC was 825.46 m2 g−1. The results of this investigation presented that RSM is a powerful statistical optimization and modeling tool for RB19 removal using adsorption process. Competing interests The authors declare that they have no competing interests. Authors’ contributions This work is part of the Master thesis of ER where MRA, Supervisor of the thesis, suggested the problem and read the paper and MR, Co-Supervisor of the thesis, helped in analysis of experiments. All authors read and approved the final manuscript. Acknowledgements The authors are grateful to the Amirkabir University of Technology (AUT) research fund for the financial support. In addition, the authors wish to express thanks to Ms. Armineh Azizi and Ms. Shabnam Sadri Moghaddam (PhD students of environmental engineering), and Ms. Lida Ezzedinloo for their assistance during experiments. Author details 1 Department of Civil and Environmental Engineering, Amirkabir University of Technology (AUT), Tehran, Iran. 2Department of Textile Engineering, Amirkabir University of Technology (AUT), Tehran, Iran. Received: 27 December 2012 Accepted: 5 March 2014 Published: 28 March 2014 References 1. Santos SCR, Boaventura RAR: Adsorption modeling of textile dyes by sepiolite. Appl Clay Sci 2008, 42:137–145. 2. Crini G: Non-conventional low-cost adsorbents for dye removal: a review. Bioresour Technol 2006, 97:1061–1085. 3. Sadri MS, Alavi Moghaddam MR, Arami M: Decolorization of an acidic dye from synthetic wastewater by sludge of water treatment plant. Iran J Environ Health Sci Eng 2010, 7:437–442. 4. Ehrampoush MH, Ghanizadeh G, Ghaneian MT: Equilibrium and kinetics study of reactive red 123 dye removal from aqueous solution by adsorption on eggshell. Iran J Environ Health Sci Eng 2011, 8:101–108. 5. Xu Y, Lebrun RE: Treatment of textile dye plant effluent by nanofiltration membrane. Separa Sci Technol 1999, 34:2501–2519. 6. Bechtold T, Burtscher E, Turcanu A: Cathodic decolorisation of textile wastewater containing reactive dyes using multi-cathode electrolyser. J Chem Technol Biotechnol 2001, 76:303–311. 7. Sadri MS, Alavi Moghaddam MR, Arami M: Coagulation/flocculation process for dye removal using sludge from water treatment plant: optimization through response surface methodology. J Hazard Mater 2010, 175:651–657. 8. Hosseini KE, Alavi Moghaddam MR, Hashemi SH: Investigation of decolorization kinetics and biodegradation of azo dye Acid Red 18 using sequential process of anaerobic sequencing batch reactor/moving bed sequencing batch biofilm reactor. Int Biodeter Biodeg 2012, 71:43–49. 9. Chatterjee S, Lee DS, Lee MW, Woo SH: Enhanced adsorption of congo red from aqueous solutions by chitosan hydrogel beads impregnated with cetyl trimethyl ammonium bromide. Bioresour Technol 2009, 100:2803–2809. 10. Samarghandi MR, Zarrabi M, Noori Sepehr M, Amrane A, Hossein Safari G, Bashiri S: Application of acidic treated pumice as an adsorbent for the removal of azo dye from aqueous solutions: kinetic, equilibrium and thermodynamic studies. Iran J Environ Health Sci Eng 2012, 9:101–108. 11. Lua AC, Yang T: Characteristics of activated carbon prepared from pistachio-nut shell by zinc chloride activation under nitrogen and vacuum conditions. J Colloid Inter Sci 2005, 290:505–513. 12. Benadjemia M, Millière L, Reinert L, Benderdouche N, Duclaux L: Preparation, characterization and Methylene Blue adsorption of phosphoric acid activated carbons from globe artichoke leaves. Fuel Process Technol 2011, 92:1203–1212.

Page 8 of 8

13. Wu FC, Wu PH, Tseng RL, Juang RS: Preparation of activated carbons from unburnt coal in bottom ash with KOH activation for liquid-phase adsorption. J Environ Manage 2010, 91:1097–1102. 14. Ravikumar K, Ramalingam S, Krishnan S, Balu K: Application of response surface methodology to optimize the process variables for reactive red and acid brown dye removal using a novel adsorbent. Dyes Pigment 2006, 70:18–26. 15. Auta M, Hameed BH: Optimized waste tea activated carbon for adsorption of methylene blue and acid blue 29 dyes using response surface methodology. Chem Eng J 2011, 175:233–243. 16. Liu Y, Wang J, Zheng Y, Wang A: Adsorption of methylene blue by kapok fiber treated by sodium chlorite optimized with response surface methodology. Chem Eng J 2012, 184:248–255. 17. Chatterjee S, Kumar A, Basu S, Dutta S: Application of response surface methodology for methylene blue dye removal from aqueous solution using low cost adsorbent. Chem Eng J 2012, 181:289–299. 18. Azizi A, Alavi Moghaddam MR, Arami M: Application of wood waste for a reactive dye removal from aqueous solutions: optimization through response surface methodology. J Environ Eng Manag. in press. 19. Liu Y, Zheng Y, Wang A: Response surface methodology for optimizing adsorption process parameters for methylene blue removal by a hydrogel composite. Adsorp Sci Technol 2010, 28:913–922. 20. Azizi A, Alavi Moghaddam MR, Arami M: Wood Waste from mazandaran wood and the paper industry as a low cost adsorbent for removal of a reactive dye. J Resid Sci Technol 2011, 8:21–28. 21. Khaled A, Nemr AE, Sikaily AE, Abdelwahab O: Removal of direct N blue106 from artificial textile dye effluent using activated carbon from orange peel: adsorption isotherm and kinetic studies. J Hazard Mater 2009, 165:100–110. 22. Mahmoodi NM, Hayati B, Arami M, Lan C: Adsorption of textile dyes on pine cone from colored wastewater: kinetic, equilibrium and thermodynamic studies. Desalination 2011, 268:117–125. 23. Sadri MS, Alavi Moghaddam MR, Aram M: A comparative study of acid red 119 dye adsorption onto dried sewage sludge and sewage sludge ash: isotherm, kinetic and desorption study. J Resid Sci Technol 2010, 7:199–207. doi:10.1186/2052-336X-12-65 Cite this article as: Radaei et al.: Removal of reactive blue 19 from aqueous solution by pomegranate residual-based activated carbon: optimization by response surface methodology. Journal of Environmental Health Science & Engineering 2014 12:65.

Submit your next manuscript to BioMed Central and take full advantage of: • Convenient online submission • Thorough peer review • No space constraints or color ﬁgure charges • Immediate publication on acceptance • Inclusion in PubMed, CAS, Scopus and Google Scholar • Research which is freely available for redistribution Submit your manuscript at www.biomedcentral.com/submit